Cancer Biol Med 2016. doi: 10.20892/j.issn.2095-3941.2016.0052
Advances in biodegradable nanomaterials for photothermal therapy of cancer Chao-Feng He1,2, Shun-Hao Wang2, Ying-Jie Yu3, He-Yun Shen2, Yan Zhao4, Hui-Ling Gao2, Hai Wang5, Lin-Lin Li6, Hui-Yu Liu2 1School
of Material Science and Engineering, Henan Polytechnic University, Jiaozuo 454000, China; 2Beijing Key Laboratory of Bioprocess, Beijing University of Chemical Technology, Beijing 100029, China; 3Department of Materials Science and Engineering, State University of New York at Stony Brook, Stony Brook, NY 11790, USA; 4Department of Emergency, Shandong Heze Municipal Hospital, Heze 274031, China; 5CAS Key Laboratory for Biomedical Effects of Nanomaterials & Nanosafety, CAS Center for Excellence in Nanoscience, National Center for Nanoscience and Technology (NCNST), Beijing 100190, China; 6Beijing Institute of Nanoenergy and Nanosystems, National Center for Nanoscience and Technology (NCNST), Chinese Academy of Sciences, Beijing 100083, China
Photothermal cancer therapy is an alternative to chemotherapy, radiotherapy, and surgery. With the development of nanophotothermal agents, this therapy holds immense potential in clinical translation. However, the toxicity issues derived from the fact that nanomaterials are trapped and retained in the reticuloendothelial systems limit their biomedical application. Developing biodegradable photothermal agents is the most practical route to address these concerns. In addition to the physicochemical properties of nanomaterials, various internal and external stimuli play key roles on nanomaterials uptake, transport, and clearance. In this review, we summarized novel nanoplatforms for photothermal therapy; these nanoplatforms can elicit stimuli-triggered degradation. We focused on the recent innovative designs endowed with biodegradable photothermal agents under different stimuli, including enzyme, pH, and near-infrared (NIR) laser. Photothermal therapy; enzyme stimuli; pH stimuli; near-infrared laser stimuli; biodegradability
Introduction Photothermal therapy (PTT), which employs photothermal agents (PTAs) to convert light to heat for the thermal ablation of cancer cells, has attracted great attention because of certain advantages, such as minimal invasiveness, high specificity, few complications, and low toxicity to normal tissues 1 . Studies have been devoted in the exploration of numerous nano-PTAs for PTT, including gold-based nanostructures 2 - 4 , conjugated polymers 5 , 6 , carbon nanomaterials (NMs)7,8, semiconductor NMs9,10, and other currently developed nano-PTAs11,12. Although most of them exhibit high therapeutic efficacy, clinical translation has been restricted because of certain concerns with regard to their long-term accumulation in the main organs, which could Correspondence to: Hui-Yu Liu E-mail: [email protected]
Received July 20, 2016; accepted August 30, 2016. Available at www.cancerbiomed.org Copyright © 2016 by Cancer Biology & Medicine
result in toxicity 13 , side effects 14 , and inflammatory response15. Our recent study evaluated the biodistribution and clearance of gold nanoshells during which polyethylene glycol (PEG)-functionalized gold nanoshells were mostly retained in the liver and spleen, even at 15 days after injection 16 . The slow clearance from these organs was consistent with the low excretion of Au content from urine and feces samples17. According to the US Food and Drug Administration (FDA), theranostic agents in clinics must be eliminated or cleared in a reasonable period of time 18 . Therefore, biodegradability and biocompatibility have become essential requirements for the clinical applications of PTAs. Novel nanoplatforms that can elicit stimuli-responsive degradation show great promise in nanoscience and nanomedicine. Biodegradable polymers are preferable because of their good biocompatibility, identified degradation mechanism, and set of metabolic pathways. Conventional methods for the preparation of stimuliresponsive polymers involve the incorporation of cleavable linkages into the main chains19 or pendant chains20. Their
long molecular chains are first ruptured by biological activity 2 1 . Then the fragmented carbon chains are metabolized by different organisms. In contrast to the organic NMs, inorganic nanoparticles have limited clinical translations because of the concerns regarding their longterm toxicity. A recent review introduced certain biodegradable inorganic materials investigated in preclinical studies22. Iron oxide nanoparticles (IONPs) have been found to release a trace element of Fe ions to the bloodstream during certain metabolic processes 23 . Porous silicon nanoparticles are degraded into water-soluble silicic acid and then are eliminated from the body in 1 week 24 . As NMs smaller than 5.5 nm can achieve renal clearance25, inorganic NMs with smaller sizes are likely degraded into nontoxic products and eliminated through the kidneys24. In view of the expanding research on PTAs, the most recent and relevant reviews have focused on the synthesis and applications of PTAs 26 . However, the processes in the biodegradation of PTAs require further research. In this review, we focused on the different types of stimuli, including those in the internal environment (enzymes, pH, and temperature) and in the external environment (light irradiation, magnetic field, and ultrasound), which are exploited to initiate the degradation of PTAs. Along with the innovative design or structure that can be subjected to biodegradation under these stimuli, the photothermal efficiency and degradation behavior were addressed. The major targeting delivery and clearance pathway of the biodegradable PTAs were discussed. Finally, we recapitulated these biodegradable PTAs and the challenges in PTT with regard to clinical application of the former.
Stimuli-responsive degradation Stimuli-responsive degradation of PTAs can decrease the accumulation and retention of PTAs in vivo through effective clearance. They undergo hydrolytic cleavage, surface oxidation, or structural fracture in response to a certain stimulus. In this section, we discuss certain of biodegradable PTAs that take advantage of various stimuli, such as enzyme, pH, and near-infrared (NIR) laser.
Enzyme-induced degradation Enzyme-catalyzed hydrolysis degradation Phospholipase A2 (PLA2) is a well-known hydrolysis agent used for recognizing and hydrolyzing the sn-2 acyl bond of phospholipids that releases free fatty acids and lysophosphatidic acid27. These enzymes are commonly found
He et al. Biodegradable nanomaterials for PTT of cancer
in mammalian tissues and are overexpressed in tumors. This unique characteristic of PLA2 can enable the use of biodegradable lipid-based structures in biomedical applications. For example, liposomes with lipid bilayers have been approved as drug carriers because of their biodegradability28. In this regard,many efforts have been made to improve their NIR absorption. Several methods to improve their NIR absorption were thus discovered, such as the loading of indocyanine green (ICG) in aqueous core29 or lipid bilayer of liposome30. In 2011, Lovell et al.31 developed a novel liposome-like structure (porphysomes) by self-assembled porphyrin analogue-lipid conjugation (1:1 molecule ratio). The porphyrin analogue (pyropheophorbide or bacteriochlorophyll) was located at the sn-2 position of the lysophosphatidylcholine (Figure 1A). Alternatively, metal ions can be inserted into the porphyrin-lipid structure to form unique metal-chelating bilayers. These liposome-like porphysomes containing approximately 80,000 porphyrins can effectively convert light into heat through the fluorescence-quenching porphyrins in the intact porphysomes. This high conversion efficiency is comparable with gold nanorods under 673 nm laser irradiation (Figure 1B). When exposed to laser (658 nm, 1.9 W/cm 2 ), the injected pyropheophorbide-porphysomes (42 mg/kg) can lead to a temperature increase (up to 60 °C), which can completely eradicate KB tumors in xenograft-bearing mice (Figure 1C). Jin et al. 32 corroborated the toxicity of the photothermal effect in tumors but not the photodynamic effect. They also found that the heat generated by the porphysomes is highly dependent on their integrated structure, and the singlet oxygen production can restore on the disrupting structure. For biodegradability, pyropheophorbide-porphysomes could degrade into the starting material when incubated with lipase, as shown in Figure 1A. The nature of the enzymatic biodegradation in vitro was likely because of the cleaving of the porphyrin by lipase in the sn-2 position of lipid33. Lovell et al.33 further confirmed the substantial degradation of pyropheophorbideporphysomes after in vivo intravenous (IV) administration. Moreover, no toxicity was observed after the introduction of pyropheophorbide-porphysomes (1,000 mg/kg) in the system, thus it is highly biocompatible. Liposome-gold clusters are another lipid-based structures formed through the assembling of gold clusters on the liposome core34. The high-density packing of gold clusters retains the NIR absorption property of the metallic shells, and the liposome scaffold provides degradability. According
Cancer Biol Med Vol 13, No 3 September 2016
Figure 1 (A) Illustration of formation and enzymatic degradation process of a pyropheophorbide-lipid porphysomes. Porphysome were assembled from the phospholipid (red) conjugated with porphyrin (blue), and degraded by incubation with detergent and lipase. (B) Photothermal images of solutions (PBS, liposome, gold nanorods, porphysomes) after 673 nm laser light irradiation. (C) Photographs of KB tumor-bearing mice after photothermal therapy using porphysomes. Reproduced with permission from Ref. 31. Copyright 2009 Nature Publishing Group.
to the literature, the destabilization of the liposome template facilitates the splitting of gold nanoparticles into small particles with a renal clearance size (5–6 nm) (Figure 2A). When the liposome-gold clusters suspension was incubated with PLA2 and Ca 2+ at 45 °C overnight, the plasmon resonance gradually disappeared and changed its color. As for the Triton X-100, the remaining suspension showed an average diameter of ~5.7 nm, indicating the degradation of the composite. Troutman et al. 34 first reported the architecture of the liposome-gold clusters based on a dialkyl phosphatidylcholine (DPPC) template. Rengan et al. 35 investigated the antitumor effects of liposome-gold clusters on MCF-7 cancer cell and performed a pharmacokinetic study on liposome-gold clusters using mice. For PTT, 15 μg/mL liposome-gold clusters can efficiently ablate cancer cells, which is indicated by the breaking of the DNA double strands under NIR laser (750 nm, 650 mW) illumination for 4 min (Figure 2B). Quantitative analysis on feces and urine samples identified the hepato-biliary and renal pathway clearance of the small particles (Figure 2C). Liposome-gold clusters tend to aggregate in the major organs and they gradually cleave into smaller particles after IV injection (Figure 2D). Apart from the enzymatic degradation, the NIR light can be used to initiate the destabilization of the
liposome-gold clusters for spatial- and temporal-controlled content release36-38.
Enzyme-catalyzed oxidation degradation Horseradish peroxidase (HRP) is among the extensively used metalloenzymes for catalytic oxidation in a variety of substrates, frequently in the presence of hydrogen peroxide (H2O2). This oxidation action is known to imitate the redox process in a cellular metabolism. In 2008, researchers discovered that single-walled carbon nanotubes (SWNTs) can be degraded by HRP in the presence of H2O2. After 12 weeks of incubation in phosphate buffered saline (PBS) at 4 °C, no distinct tubular structure of carbon nanotubes were observed, thereby indicating that nearly all nanotube materials were degraded 39 . To further investigate the mechanism of HRP-catalyzed degradation, Allen et al. 40 compared the degradation course of the carboxylated SWNTs and the pristine SWNTs using HRP and H2O2. Their data suggested that the hydrophobic surface on pristine SWNTs were resistant to the HRP catalyst, whereas the carboxylated sites on the SWNTs facilitated the adsorption of HRP, thereby enhancing the catalytic effect. Moreover, the degraded products gradually evolved from oxidized aromatic fragments to CO 2 . These results can be extended to the
He et al. Biodegradable nanomaterials for PTT of cancer
Figure 2 (A) Illustration of the formation and degradation processes of liposome-gold clusters (LiposAu). (B) Fluorescence micrograph images of MCF-7 cancer cell after photothermal effect (750 nm, 2.3 w/cm2, 4 min) induced by liposome-gold clusters (15 μg/mL). Red color represents TurboFP fluorescent protein overexpressed in cancer cells. (C) Tissue biodistribution of Au in vivo at different days after IV injection of liposome-gold clusters. (D) TEM of kidney tissue without any treatment (i), and with liposome-gold clusters NP (ii). Liposomegold clusters are cleaved into small gold nanoparticles less than 5 nm (iii). Reproduced with permission from Ref. 35. Copyright 2015 American Chemical Society.
degradation of SWNTs in living systems 41-44 . When incubated with neutrophils and macrophages, the SWNTs were also degraded by myeloperoxidase. Particularly, the SWNTs first produced defects in the outer wall, and the developed defects initiated structure alterations over increased incubation time41. Moreover, the experiments on mice proved in vivo that the oxidative biodegradation of SWNTs is associated to human myeloperoxidase42. Some researchers also reported that SWNTs can be degraded in the brain cortex 45 and in the primary microglial culture models 4 6 . They emphasized that the defects or the functionalized sites on carbon nanotubes significantly facilitate enzymatic action. HRP-induced degradation of multiwalled carbon nanotubes with defective sites in the graphitic walls was demonstrated by Zhao et al.47. Carbon nanotubes cancer mediate photothermal tumor destruction
which has been documented in several studies48-53, but their slow degradation rate in vivo and their degradation byproduct such as reactive oxygen species 43,44 are still unsuitable for clinical application. The structural design and surface functionalization that exposed more active sites (carboxylic groups, defects) on the graphitic surface could accelerate this enzymatic degradation. Graphene oxide (GO) is another graphite derivative that have shown great potential for biological applications in photothermal therapy and drug delivery. The development of biodegradable GOs is of great importance, and can promote the development of nanomedicine. As GOs have similar sp2 allotropes of carbon similar to carbon nanotubes, they were also reported to be able to undergo similar HRP-induced oxidative degradation in the presence of H2O254. Figure 3A shows the molecular modeling of an HRP on a GO. Because
Cancer Biol Med Vol 13, No 3 September 2016
Figure 3 (A) Illustration of the binding position of HRP on graphene oxide, holey graphene oxide, and a small sheet of graphene oxide (from left to right). (B) TEM image of graphene oxide incubated with solution containing HRP and 40 μM H2O2 after 0, 5, 10 days. (C) Atomic force microscopy (AFM) images of graphene oxide incubated with HRP after 0 day and 10 days. The sheet heights of the graphene oxide in day 0 and day 10 are 9.81 nm and 1.10 nm, respectively. Reproduced with permission from Ref. 54. Copyright 2011 American Chemical Society.
of the effect of the HRP, the basal plane of the GO gradually produced certain holes, which can act as cleavage sites for carbon-carbon bonds. This result is consistent with the observations in the transmission electron microscopy (TEM) images (Figure 3B) and atomic force microscopy (AFM) images (Figure 3C). Afterward,a gradual tendency of graphene to disorganize its structure in vivo was observed at the 3rd month after injection. This process was related to the processes of the tissue-bound macrophages. However, the problems of long-term retention still cannot be addressed, which lead to toxicity risks and immune response 55 . To improve its biocompatibility, GO is usually functionalized with PEG or bovine serum albumin (BSA), producing PEGGO and BSA-GO. However, PEG-GO and BSA-GO cannot degrade in HRP and H2O2 because the PEG or BSA in the GO surface inhibits the interaction between the HRP and GO56. When GO was functionalized with a cleavable PEG (mPEG-SS-NH 2 ), the generated GO-SS-PEG cleaved the disulfide linkages by dithiothreitol, resulting in the
degradation in HRP and H2O256. Similarly, the GO-SS-PEG degradation in A549 cells can be triggered by a high concentration of glutathione57.
pH-induced degradation The interstitial pH of tumor tissues is ~6.8, which is lower than that of the normal tissues (pH=7.2–7.4). Moreover the endosomes and lysosomes show lower pH levels (pH